• date post

17-Jun-2020
• Category

## Documents

• view

18

1

Embed Size (px)

### Transcript of Dynamic Mechanical Analysis (DMA) Basics and Beyond ring/ChE 5655 Chip Processing... ·...

• Dynamic Mechanical Analysis (DMA) Basics and Beyond

Dr. Lin Li Thermal Analysis PerkinElmer Inc.

April 2000

ε∗ ω= Σ(∆εβ/1+ιωτβ)

• molecular structure

processing conditions

product properties

Material Behavior

The DMA lets you relate:

• Force Motor

Temperature Enclosure

LVDT

Core Rod

Interchangeable

Furnace Heat Sink/Cooling System

Measuring System

How the DMA works:

DMA Structure in general

Coil Magnet

!Constant inputs and outputs function as in the TMA

!A sine wave current is added to the force coil

!The resultant sine wave voltage of the LVDT is compared to the sine wave force

!The amplitude of the LVDT is related to the storage modulus, E' via the spring constant, k.

!The phase lag, δ, is related to the E" via the damping constant, D.

• Outstanding Flexibility 1: Multiple Geometries

Extension

Compressive Shear

Flexure

Parallel Plate Cup & Plate Tray & Plate Sintered Plates 3 pt. Bending 4 pt. Bending ASTM Flexure Dual Cantilever Single Cantilever Extension Shear Sandwich Coaxial Cylinder Paper FoldCup & Plate

• Why?

3 4 5 6 7 8 9 10 11 12

Lo g

E ’

1 mm

20 mm

20 mm

5 mm

• Stress Causes Strain...

Lo L

Cauchy or Engineering Strain

L-Lo = ∆L

Henchy or True Strain εεεε = ln (∆L/Lo)

εεεε = ∆L/Lo

Kinetic Theory of Rubber Strain εεεε = 1/3{L/Lo-(Lo/L)2}

Kirchhoff Strain

Murnaghan Strain

εεεε = 1/2{ (L/Lo)2-1}

εεεε = 1/2{1-(Lo/L)2}

The different definitions of tensile strain become equivalent at very small deformations.

• The Elastic Limit: Hooke’s Law

=

Strain increases with increasing

Stress

σσσσ

ε ε ε ε

slope = k

• Real vs... Hookean Stress- Strain Curves

4.0 8.0 12.0 16.0

0.0

0.2

0.4

0.6

0.8

1.0

1.2

1.4

Thu Apr 14 16:34:38 1994

Slope 359171.32 Pa/%

St re

ss (P

a x

10 7 )

KPMStrain (%)

Slope 1642965.02 Pa/%

Curve 1: DMA Creep Recoveryin Parallel Plate File info: Drssr90R.2Thu Apr 14 15:16:52 1994 Sample Height:3.359 mmCreep Stress: 2600.0mN Recovery Stress: 1.0mN Dresser 90 Durameter

PERKIN-ELMER 7 Series ThermalAnalysis System

TEMP1: 20.0 C TIME1: 5.3 min

Limiting Modulus

Real behavior

Hookean Behavior

σσσσ

εεεε

• The Viscous Limit: Newtonian Behavior

σσσσ

γ γ γ γ .

The speed at which the fluid flows through the holes (the strain rate)

increases with stress!!!

slope = η

• Viscosity Effects • Newtonian behavior is linear and the

viscosity is independent of rate. • Pseudoplastic fluids get thinner as shear

increases. • Dilatant Fluids increase their viscosity as

shear rates increase. • Plastic Fluids have a yield point with

pseudoplastic behavior. • Thixotrophic and rheopectic fluids show

viscosity-time nonlinear behavior. For example, the former shear thin and then reform its gel structure.

γ γ γ γ

ττττ

.

• Polymers are Non-Newtonian Fluids!!!

• At low shear rates, the viscosity is controlled by MW. The material shows Newtonian behavior

• Viscosity shows a linear dependence on rate above the ηo region.

• At high rates, the material can no longer shear thin and a second plateau is reached.

η ηηη

γγγγ.

Zero Shear Plateau ~ ηηηηo

Infinite Shear Plateau ~ ηηηη∞

Linear Dependence on Rate

Lo g

Log

• Analyzing a Stress-Strain Curve

σσσσ

εεεε

linear region nonlinear region

failure (εΒ, σΒ)

yield point (εy, σy)

Young’s modulus (E) E d

d L

L

= =σ ε

σ ε

The area under the curve to this line is the energy needed to break the material

• Under Continuos Loads: Creep Recovery

• Applying a constant load for long times and removing it from a sample.

• Allows one to see the distortion under constant load and also how well it recovers.

• Creep is a fundamental engineering test.

• Creep is used as a basic test for design.

• By looking at both the creep and recovery parts of the curve, we can begin to examine how polymers relax.

0.0 1.0 2.0 3.0 4.0 5.0 6.0 7.0 0.0000

0.0005

0.0010

0.0015

0.0020

0.0025

-250.0

0.0

250.0

500.0

750.0

1000.0

1250.0

1500.0

1750.0

2000.0

2250.0

2500.0

Thu Apr 28 20:32:20 1994

St ra

in (%

)

DMA7 APPLICATIONS LABTime (minutes)

# 1 PTFE - CREEP/RELAXATION AT -5C:cr_ptfe-5 Strain (%)

Curve 1: DMA Creep Recoveryin 3 Point Bending File info: cr_ptfe-5 Wed Jun 29 15:31:18 1988 Sample Height:3.300mmCreep Stress: 1.50e+06Pa Recovery Stress: 6.25e+02Pa PTFE - CREEP/RELAXATION

PERKIN-ELMER 7 Series ThermalAnalysis System

TEMP1: -15.0 C TIME1: 7.0 min

Fo rc

e (m

N )

# 2 Force (mN)

• Dynamic Stress

F (static)

Force

Time

Force (dynamic)

Phase angle = δ= δ= δ= δ

Stress

Time

material response

Strain =yo/y

Amplitude = k

Stress =FA

• Why? Let’s bounce a ball.

E” ~ energy loss in internal motion

E’ ~ elastic response

• All this is calculated from δ δ δ δ and k:

• From k, we calculate E’ (storage modulus) • From δ, we calculate E’’ (loss modulus) • then:

Tan δ = E”/E’ E* = E’ + iE” = SQRT(E’2 + E”2) G* = E*/2(1+ν) η = 3G*/ω

• To apply this to materials...

σσσσοοοο

ε ε ε ε οοοο

Dynamic Stress Scan Since each part of the ramp has a sine wave stress associated with it, we get:

tan δ E*, E’, E” η

for each data point!!εεεεσσσσ

• For example, DSS Curves

0.2 0.4 0.6 0.8 1.0

1.0

1.5

2.0

2.5

3.0

3.5

4.0

4.5

5.0

5.5

Thu Apr 28 20:28:00 1994

V is

co si

ty (P

a s

x 10

7 )

KPMStrain (%)

# 1 Dresser 70 Durameter:Drssr70Dss Complex Viscosity (Pa s x 10 7)

Curve 1: DMA AC Stress Scanin Parallel Plate File info: Drssr70DssThu Apr 14 16:44:41 1994 Frequency: 1.00 Hz Stress Rate: 250.0mN/min

Tension: 110.000% Dresser 70 Durameter

PERKIN-ELMER 7 Series ThermalAnalysis System

TEMP1: 10.5 C TIME1: -1.2 min

Complex Viscosity (Pa s x 10 7)

0.2 0.4 0.6 0.8 1.0 0.0

0.5

1.0

1.5

2.0

2.5

3.0

3.5

4.0

4.5

5.0

5.5

Thu Apr 14 16:59:58 1994

D yn

am ic

S tre

ss (P

a x

10 6 )

KPMStrain (%)

Slope 1274361.04 Pa/%

Curve 1: DMA AC Stress Scanin Parallel Plate File info: Drssr70DssThu Apr 14 16:44:41 1994 Frequency: 1.00 Hz Stress Rate: 250.0mN/min

Tension: 110.000% Dresser 70 Durameter

PERKIN-ELMER 7 Series ThermalAnalysis System

TEMP1: 10.5 C TIME1: -1.2 min

Slope 6297938.16 Pa/%

• Now, let’s induce temperature as a variable.

• We can heat the material under minimal load at a calibrated rate.

• This allows the material to change with temperature.

• These changes can be described in terms of free volume or relaxation times.

Fr ee

V ol

um e

• Thermomechanical Analysis as a starting Point.

50.0 75.0 100.0 125.0 150.0 175.0 0.0

0.5

1.0

1.5

2.0

2.5

3.0

3.5

4.0

4.5

5.0

5.5

6.0

6.5

7.0

Sun Nov 26 20:10:47 1995

Pe ne

tra tio

n (m

m )

Temperature (C)

# 1 Tg by flex:Tgflex Penetration (mm)

Onset 106.92 C

Curve 1: TMA in Penetration File info: Tgflex Tue Oct 10 16:21:08 1995

DC Force: 100.0 mNSample Height:4.180 mm Tg by flex

PERKIN-ELMER 7 Series Thermal Analysis System

TEMP1: 30.0 C TIME1: 0.0 min RATE1: 10.0 C/min TEMP2: 150.0 C

• TMA - It’s all free volume.

70.0 80.0 90.0 100.0 110.0

1.70

1.75

1.80

1.85

1.90

1.95

2.00

2.05

2.10

Sun Nov 26 20:08:09 1995

Ex pa

ns io

n (m

m )

Temperature ( C)

# 1 cte :cte Expansion (mm)

Onset 105.53 C Cx 2.948 x 10 -5 / C

Cx 2.19